Phosphide‒Tetrahedrite Ag6Ge10P12: Thermoelectric Performance of a Long-Forgotten Silver-Cluster Compound
Nuss, Jürgen; Wedig, Ulrich; Xie, Wenjie; Yordanov, Petar; Bruin, Jan; Hübner, Ralph; Weidenkaff, Anke; Takagi, Hidenori; Chemistry of Materials 29 (2017) 6956–; doi:10.1021/acs.chemmater.7b02474

data_4002840
_publ_section_title
;
 Phosphide--Tetrahedrite Ag6Ge10P12: Thermoelectric Performance of a
 Long-Forgotten Silver-Cluster Compound
;
_journal_issue                   16
_journal_name_full               'Chemistry of Materials'
_journal_page_first              6956
_journal_paper_doi               10.1021/acs.chemmater.7b02474
_journal_volume                  29
_journal_year                    2017
_chemical_absolute_configuration ad
_chemical_formula_moiety         'Ag6 Ge10 P12'
_chemical_formula_sum            'Ag6 Ge10 P12'
_chemical_formula_weight         1744.76
_space_group_crystal_system      cubic
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      217
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.3004(15)
_cell_length_b                   10.3004(15)
_cell_length_c                   10.3004(15)
_cell_measurement_reflns_used    3644
_cell_measurement_temperature    100.0(2)
_cell_measurement_theta_max      34.83
_cell_measurement_theta_min      2.79
_cell_volume                     1092.9(3)
_computing_cell_refinement       'SAINT32 (Bruker AXS)'
_computing_data_collection       'Bruker Suite (Bruker AXS)'
_computing_data_reduction        'SAINT32 (Bruker AXS)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100.0(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'SMART APEX, Bruker AXS'
_diffrn_measurement_method       \wscan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0414
_diffrn_reflns_av_unetI/netI     0.0167
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            8545
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.986
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         35.261
_diffrn_reflns_theta_min         2.797
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    19.633
_exptl_absorpt_correction_T_max  0.273
_exptl_absorpt_correction_T_min  0.173
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
semi empirical absorption correction with SADABS,
G.M. Sheldrick, SADABS, Version 2012/1, University of G\"ottingen. Germany. 
;
_exptl_crystal_colour            'silver grey'
_exptl_crystal_density_diffrn    5.302
_exptl_crystal_description       block
_exptl_crystal_F_000             1564
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.030
_refine_diff_density_max         1.551
_refine_diff_density_min         -0.907
_refine_diff_density_rms         0.210
_refine_ls_abs_structure_details
;
 Flack x determined using 200 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons and Flack (2004), Acta Cryst. A60, s61).
;
_refine_ls_abs_structure_Flack   0.013(12)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.213
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     16
_refine_ls_number_reflns         489
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.213
_refine_ls_R_factor_all          0.0235
_refine_ls_R_factor_gt           0.0217
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0166P)^2^+8.7517P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0463
_refine_ls_wR_factor_ref         0.0493
_reflns_Friedel_coverage         0.765
_reflns_Friedel_fraction_full    0.989
_reflns_Friedel_fraction_max     0.981
_reflns_number_gt                467
_reflns_number_total             489
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm7b02474_si_004.cif
_cod_data_source_block           Ag6ge10P12_100K
_cod_original_cell_volume        1092.9(5)
_cod_database_code               4002840
_shelx_estimated_absorpt_t_min   0.202
_shelx_estimated_absorpt_t_max   0.590
_shelxl_version_number           2013-4
_shelx_res_checksum              77280
_shelx_hkl_checksum              56283